General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 7.76 g/cm³ Show Material materials with Density of 7.76 g/cm³ |

50.0 °C | 7.75 g/cm³ Show Material materials with Density of 7.75 g/cm³ | |

100.0 °C | 7.74 g/cm³ Show Material materials with Density of 7.74 g/cm³ | |

150.0 °C | 7.73 g/cm³ Show Material materials with Density of 7.73 g/cm³ | |

200.0 °C | 7.71 g/cm³ Show Material materials with Density of 7.71 g/cm³ | |

250.0 °C | 7.7 g/cm³ Show Material materials with Density of 7.7 g/cm³ | |

300.0 °C | 7.68 g/cm³ Show Material materials with Density of 7.68 g/cm³ | |

350.0 °C | 7.67 g/cm³ Show Material materials with Density of 7.67 g/cm³ | |

400.0 °C | 7.65 g/cm³ Show Material materials with Density of 7.65 g/cm³ | |

450.0 °C | 7.64 g/cm³ Show Material materials with Density of 7.64 g/cm³ | |

500.0 °C | 7.62 g/cm³ Show Material materials with Density of 7.62 g/cm³ | |

550.0 °C | 7.61 g/cm³ Show Material materials with Density of 7.61 g/cm³ | |

600.0 °C | 7.59 g/cm³ Show Material materials with Density of 7.59 g/cm³ | |

Mechanical

Property | Temperature | Value |
---|---|---|

Elastic modulus | 20.0 °C | 217.68 - 218 GPa Show Material materials with Elastic modulus of 217.68 - 218 GPa |

50.0 °C | 216.02 GPa Show Material materials with Elastic modulus of 216.02 GPa | |

100.0 °C | 212.98 - 213 GPa Show Material materials with Elastic modulus of 212.98 - 213 GPa | |

150.0 °C | 209.64 GPa Show Material materials with Elastic modulus of 209.64 GPa | |

200.0 °C | 206 - 206.21 GPa Show Material materials with Elastic modulus of 206 - 206.21 GPa | |

250.0 °C | 202.38 GPa Show Material materials with Elastic modulus of 202.38 GPa | |

300.0 °C | 198 - 198.26 GPa Show Material materials with Elastic modulus of 198 - 198.26 GPa | |

350.0 °C | 193.94 GPa Show Material materials with Elastic modulus of 193.94 GPa | |

400.0 °C | 189 - 190 GPa Show Material materials with Elastic modulus of 189 - 190 GPa | |

450.0 °C | 184.33 GPa Show Material materials with Elastic modulus of 184.33 GPa | |

500.0 °C | 178.93 - 180 GPa Show Material materials with Elastic modulus of 178.93 - 180 GPa | |

550.0 °C | 172.85 GPa Show Material materials with Elastic modulus of 172.85 GPa | |

600.0 °C | 165.79 - 167 GPa Show Material materials with Elastic modulus of 165.79 - 167 GPa | |

Unlock all property charts | ||

Elongation | 20.0 °C | 16 - 17 % Show Material materials with Elongation of 16 - 17 % |

Elongation, transverse | 20.0 °C | 14 % Show Material materials with Elongation, transverse of 14 % |

Poisson's ratio | 20.0 °C | 0.28 [-] Show Material materials with Poisson's ratio of 0.28 [-] |

50.0 °C | 0.28 [-] Show Material materials with Poisson's ratio of 0.28 [-] | |

100.0 °C | 0.28 [-] Show Material materials with Poisson's ratio of 0.28 [-] | |

150.0 °C | 0.28 [-] Show Material materials with Poisson's ratio of 0.28 [-] | |

200.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

250.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

300.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

350.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | |

400.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

450.0 °C | 0.3 [-] Show Material materials with Poisson's ratio of 0.3 [-] | |

500.0 °C | 0.31 [-] Show Material materials with Poisson's ratio of 0.31 [-] | |

550.0 °C | 0.31 [-] Show Material materials with Poisson's ratio of 0.31 [-] | |

600.0 °C | 0.31 [-] Show Material materials with Poisson's ratio of 0.31 [-] | |

Unlock all property charts | ||

Shear modulus | 20.0 °C | 84.95 GPa Show Material materials with Shear modulus of 84.95 GPa |

50.0 °C | 84.27 GPa Show Material materials with Shear modulus of 84.27 GPa | |

100.0 °C | 82.99 GPa Show Material materials with Shear modulus of 82.99 GPa | |

150.0 °C | 81.62 GPa Show Material materials with Shear modulus of 81.62 GPa | |

200.0 °C | 80.05 GPa Show Material materials with Shear modulus of 80.05 GPa | |

250.0 °C | 78.48 GPa Show Material materials with Shear modulus of 78.48 GPa | |

300.0 °C | 76.71 GPa Show Material materials with Shear modulus of 76.71 GPa | |

350.0 °C | 74.95 GPa Show Material materials with Shear modulus of 74.95 GPa | |

400.0 °C | 73.08 GPa Show Material materials with Shear modulus of 73.08 GPa | |

450.0 °C | 70.93 GPa Show Material materials with Shear modulus of 70.93 GPa | |

500.0 °C | 68.57 GPa Show Material materials with Shear modulus of 68.57 GPa | |

550.0 °C | 66.02 GPa Show Material materials with Shear modulus of 66.02 GPa | |

600.0 °C | 63.27 GPa Show Material materials with Shear modulus of 63.27 GPa | |

Unlock all property charts | ||

Tensile strength | 20.0 °C | 690 - 850 MPa Show Material materials with Tensile strength of 690 - 850 MPa |

100.0 °C | 650 MPa Show Material materials with Tensile strength of 650 MPa | |

150.0 °C | 625 MPa Show Material materials with Tensile strength of 625 MPa | |

200.0 °C | 600 MPa Show Material materials with Tensile strength of 600 MPa | |

250.0 °C | 590 MPa Show Material materials with Tensile strength of 590 MPa | |

300.0 °C | 580 MPa Show Material materials with Tensile strength of 580 MPa | |

350.0 °C | 545 MPa Show Material materials with Tensile strength of 545 MPa | |

400.0 °C | 510 MPa Show Material materials with Tensile strength of 510 MPa | |

450.0 °C | 455 MPa Show Material materials with Tensile strength of 455 MPa | |

500.0 °C | 400 MPa Show Material materials with Tensile strength of 400 MPa | |

550.0 °C | 325 MPa Show Material materials with Tensile strength of 325 MPa | |

Unlock all property charts | ||

Tensile strength, transverse | 20.0 °C | 690 - 850 MPa Show Material materials with Tensile strength, transverse of 690 - 850 MPa |

Yield strength Rp0.2 | 20.0 °C | 490 - 500 MPa Show Material materials with Yield strength Rp0.2 of 490 - 500 MPa |

100.0 °C | 460 MPa Show Material materials with Yield strength Rp0.2 of 460 MPa | |

150.0 °C | 445 MPa Show Material materials with Yield strength Rp0.2 of 445 MPa | |

200.0 °C | 430 MPa Show Material materials with Yield strength Rp0.2 of 430 MPa | |

250.0 °C | 415 MPa Show Material materials with Yield strength Rp0.2 of 415 MPa | |

300.0 °C | 390 MPa Show Material materials with Yield strength Rp0.2 of 390 MPa | |

350.0 °C | 380 MPa Show Material materials with Yield strength Rp0.2 of 380 MPa | |

400.0 °C | 360 MPa Show Material materials with Yield strength Rp0.2 of 360 MPa | |

450.0 °C | 330 MPa Show Material materials with Yield strength Rp0.2 of 330 MPa | |

500.0 °C | 290 MPa Show Material materials with Yield strength Rp0.2 of 290 MPa | |

550.0 °C | 250 MPa Show Material materials with Yield strength Rp0.2 of 250 MPa | |

600.0 °C | 160 MPa Show Material materials with Yield strength Rp0.2 of 160 MPa | |

Unlock all property charts | ||

Yield strength Rp0.2, transverse | 20.0 °C | 490 - 500 MPa Show Material materials with Yield strength Rp0.2, transverse of 490 - 500 MPa |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | 20.0 °C | 1.02E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.02E-5 1/K | |

100.0 °C | 1.05E-5 - 1.08E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.05E-5 - 1.08E-5 1/K | ||

200.0 °C | 1.09E-5 - 1.12E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.09E-5 - 1.12E-5 1/K | ||

300.0 °C | 1.13E-5 - 1.16E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.13E-5 - 1.16E-5 1/K | ||

400.0 °C | 1.16E-5 - 1.19E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.16E-5 - 1.19E-5 1/K | ||

500.0 °C | 1.2E-5 - 1.21E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.2E-5 - 1.21E-5 1/K | ||

600.0 °C | 1.22E-5 - 1.23E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.22E-5 - 1.23E-5 1/K | ||

Unlock all property charts | |||

Max service temperature, long | 0 - 600 °C Show Material materials with Max service temperature, long of 0 - 600 °C | ||

Melting point | 1370 - 1530 °C Show Material materials with Melting point of 1370 - 1530 °C | Typical for Martensitic Stainless Steel | |

Specific heat capacity | 20.0 °C | 439 J/(kg·K) Show Material materials with Specific heat capacity of 439 J/(kg·K) | |

100.0 °C | 474 - 490 J/(kg·K) Show Material materials with Specific heat capacity of 474 - 490 J/(kg·K) | ||

200.0 °C | 498 - 540 J/(kg·K) Show Material materials with Specific heat capacity of 498 - 540 J/(kg·K) | ||

300.0 °C | 517 - 580 J/(kg·K) Show Material materials with Specific heat capacity of 517 - 580 J/(kg·K) | ||

400.0 °C | 538 - 630 J/(kg·K) Show Material materials with Specific heat capacity of 538 - 630 J/(kg·K) | ||

500.0 °C | 564 - 710 J/(kg·K) Show Material materials with Specific heat capacity of 564 - 710 J/(kg·K) | ||

600.0 °C | 598 - 830 J/(kg·K) Show Material materials with Specific heat capacity of 598 - 830 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 24 W/(m·K) Show Material materials with Thermal conductivity of 24 W/(m·K) | |

100.0 °C | 24 - 24.4 W/(m·K) Show Material materials with Thermal conductivity of 24 - 24.4 W/(m·K) | ||

200.0 °C | 24.8 - 25 W/(m·K) Show Material materials with Thermal conductivity of 24.8 - 25 W/(m·K) | ||

300.0 °C | 25 - 25.1 W/(m·K) Show Material materials with Thermal conductivity of 25 - 25.1 W/(m·K) | ||

400.0 °C | 25.6 - 26 W/(m·K) Show Material materials with Thermal conductivity of 25.6 - 26 W/(m·K) | ||

500.0 °C | 26 - 26.1 W/(m·K) Show Material materials with Thermal conductivity of 26 - 26.1 W/(m·K) | ||

600.0 °C | 26 - 26.4 W/(m·K) Show Material materials with Thermal conductivity of 26 - 26.4 W/(m·K) | ||

Unlock all property charts | |||

Thermal diffusivity | 20.0 °C | 7.1 mm²/s Show Material materials with Thermal diffusivity of 7.1 mm²/s | |

100.0 °C | 6.3 mm²/s Show Material materials with Thermal diffusivity of 6.3 mm²/s | ||

200.0 °C | 6 mm²/s Show Material materials with Thermal diffusivity of 6 mm²/s | ||

300.0 °C | 5.7 mm²/s Show Material materials with Thermal diffusivity of 5.7 mm²/s | ||

400.0 °C | 5.4 mm²/s Show Material materials with Thermal diffusivity of 5.4 mm²/s | ||

500.0 °C | 4.9 mm²/s Show Material materials with Thermal diffusivity of 4.9 mm²/s | ||

600.0 °C | 4.1 mm²/s Show Material materials with Thermal diffusivity of 4.1 mm²/s | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 6.03E-7 Ω·m Show Material materials with Electrical resistivity of 6.03E-7 Ω·m |

50.0 °C | 6.26E-7 Ω·m Show Material materials with Electrical resistivity of 6.26E-7 Ω·m | |

100.0 °C | 6.68E-7 - 6.7E-7 Ω·m Show Material materials with Electrical resistivity of 6.68E-7 - 6.7E-7 Ω·m | |

150.0 °C | 7.06E-7 Ω·m Show Material materials with Electrical resistivity of 7.06E-7 Ω·m | |

200.0 °C | 7.4E-7 - 7.43E-7 Ω·m Show Material materials with Electrical resistivity of 7.4E-7 - 7.43E-7 Ω·m | |

250.0 °C | 7.83E-7 Ω·m Show Material materials with Electrical resistivity of 7.83E-7 Ω·m | |

300.0 °C | 8.17E-7 - 8.2E-7 Ω·m Show Material materials with Electrical resistivity of 8.17E-7 - 8.2E-7 Ω·m | |

350.0 °C | 8.54E-7 Ω·m Show Material materials with Electrical resistivity of 8.54E-7 Ω·m | |

400.0 °C | 8.9E-7 Ω·m Show Material materials with Electrical resistivity of 8.9E-7 Ω·m | |

450.0 °C | 9.25E-7 Ω·m Show Material materials with Electrical resistivity of 9.25E-7 Ω·m | |

500.0 °C | 9.6E-7 - 9.62E-7 Ω·m Show Material materials with Electrical resistivity of 9.6E-7 - 9.62E-7 Ω·m | |

550.0 °C | 9.99E-7 Ω·m Show Material materials with Electrical resistivity of 9.99E-7 Ω·m | |

600.0 °C | 1.03E-6 - 1.04E-6 Ω·m Show Material materials with Electrical resistivity of 1.03E-6 - 1.04E-6 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Carbon | 0.17 - 0.23 % Show Material materials with Carbon of 0.17 - 0.23 % |

Chromium | 10 - 12.5 % Show Material materials with Chromium of 10 - 12.5 % |

Manganese | 1 % Show Material materials with Manganese of 1 % |

Molybdenum | 0.8 - 1.2 % Show Material materials with Molybdenum of 0.8 - 1.2 % |

Nickel | 0.3 - 0.8 % Show Material materials with Nickel of 0.3 - 0.8 % |

Phosphorus | 0.03 % Show Material materials with Phosphorus of 0.03 % |

Silicon | 0.5 % Show Material materials with Silicon of 0.5 % |

Sulfur | 0.03 % Show Material materials with Sulfur of 0.03 % |

Vanadium | 0.25 - 0.35 % Show Material materials with Vanadium of 0.25 - 0.35 % |